AN ABSTRACT OF THE THESIS OF Thomas J. Wright for the degree of Master of Science in Mechanical Engineering presented on November 20, 2012 Title: Sensitivity of Hashin damage parameters for notched composite panels in tension and out-of-plane bending Abstract approved: John P. Parmigani When using Finite Element Analysis (FEA) to model notched composite panels, the values of certain material properties can have a great effect on the outcome of the simulation. Progressive damage modeling is used to model how a composite structure will fail, and how that failure will affect the response of the structure. Many different progressive damage models exist, but the formulation known as Hashin damage is used to model failure in tension and out-of-plane bending in this study. This model has ten different material properties that are used to define the damage response of the material. Each of these material properties must be calculated experimentally in a time consuming and expensive process. A method of determining which properties will have the greatest effect on the model, and therefore, which to spend the most money on accurate tests, is a factorial analysis sensitivity study. Studies of this nature have been used in many different situations regarding material properties testing and optimization. The work presented in this study uses several factorial analysis designs to perform a sensitivity study on the ten Hashin damage parameters in a variety of situations. Five different ply layups are used in modeling specimens that are loaded in tension and out-of-plane bending. The results of this study show that the significant factors depend on the ply layup and loading scenario, but there are generally less than three factors that play a significant role in modeling the failure of the panels. This means that in most cases, rather than spending substantial money on finding ten different material properties, the time and money can be focused on a small subset of the properties, and an accurate model can still be achieved. While the results of the scenarios presented may not apply to all scenarios, the methods presented can be used to perform a similar study in other specific scenarios to find the significant factors for that case. ©Copyright by Thomas J. Wright November 20, 2012 All Rights Reserved Sensitivity of Hashin damage parameters for notched composite panels in tension and out-of-plane bending By Thomas J. Wright A THESIS Submitted to Oregon State University in partial fulfillment of the requirements of the degree of Master of Science Presented 20 November 2012 Commencement June 2013 Master of Science thesis of Thomas J. Wright presented on November 20, 2012 APPROVED: Major Professor, representing Mechanical Engineering Head of the School of Mechanical, Industrial, and Manufacturing Engineering Dean of Graduate School I understand that my thesis will become part of the permanent collection of Oregon State University libraries. My signature below authorizes release of my thesis to any reader upon request. Thomas J. Wright, Author ACKNOWLEDGEMENTS I would like to thank Dr. John P. Parmigiani for all of his advice and help with making this project possible. This document would not be the same without his guidance and support. He has been a great resource not only with this project, but with my entire graduate experience. His help and encouragement have been vital to my success. Each of my fellow graduate students in the Computational Mechanics and Applied Design research group has been an excellent resource. They spent countless hours in the office, and were there and available to bounce ideas off of throughout the entire research and writing process. My thanks goes out to them as well. I would also like to thank Dr. David Kim for his assistance with interpreting my results. His expertise in Design of Experiments has helped to make the results of this project worthwhile. His willingness to meet over and over again to clarify my confusion was a great help. TABLE OF CONTENTS Page 1.0 Introduction ......................................................................................................... 1 1.1 Numerical Modeling of Composites ............................................................... 1 1.2 Sensitivity Studies ........................................................................................... 5 1.3 Literature Review ............................................................................................ 6 1.4 Topic of this Work .......................................................................................... 6 2.0 Progressive Damage Model .............................................................................. 11 2.1 Hashin Damage Initiation .............................................................................. 11 2.2 Abaqus Energy-Based Damage Evolution .................................................... 12 3.0 Methods ............................................................................................................. 17 3.1 Finite Element Model .................................................................................... 17 3.2 Factorial Analysis .......................................................................................... 23 4.0 Results ............................................................................................................... 30 4.1 In-Plane Tension............................................................................................ 31 4.2 Out-of-Plane Bending.................................................................................... 54 5.0 Discussion ......................................................................................................... 71 6.0 Conclusion ........................................................................................................ 73 7.0 Bibliography...................................................................................................... 76 Appendix A: Fractional Factorial Designs ................................................................... 80 Appendix B: Results for Each Factorial Analysis........................................................ 88 Appendix C: Calculated Effects for Each Analysis ..................................................... 93 TABLE OF FIGURES Page Figure 1: Equivalent stress versus equivalent displacement (adapted from [31]) ....... 14 Figure 2: Mesh of finite element model ....................................................................... 18 Figure 3: Boundary conditions for specimen loaded in tension ................................... 19 Figure 4: Boundary conditions for specimen loaded in bending ................................. 19 Figure 5: Physical bending apparatus for proprietary testing [5] ................................. 20 Figure 6: Normal plot example showing significant factors [34] ................................ 30 Figure 7: Typical loading of tensile specimen ............................................................. 32 Figure 8: Normal probability plot of effects for Layup 1, [08], loaded in tension ....... 33 Figure 9: Normal probability plot for 23 factorial analysis for Layup 1, [08], loaded in tension ................................................................ 35 Figure 10: Runs at nominal level, with significant factors increased and others at nominal level, and with insignificant factors increased and significant factors at nominal level for Layup 1, [08], loaded in tension .............. 36 Figure 11: Normal probability plot of effects for Layup 2, [(0/45)2]s, loaded in tension ..................................................................... 37 Figure 12: Normal probability plot for 23 factorial analysis for Layup 2, [(0/45)2]s, loaded in tension ....................................................... 38 Figure 13: Runs at nominal level, with significant factors increased, and with insignificant factors increased for Layup 2, [(0/45)2]s, loaded in tension .................... 40 Figure 14: Normal probability plot of effects for Layup 3, [(-45/45)2]s, loaded in tension ................................................................. 41 TABLE OF FIGURES (continued) Page Figure 15: Normal probability plot for 26-1 factorial analysis for Layup 3, [(-45/45)2]s, loaded in tension ................................................... 42 Figure 16: (a) Interaction plot for SL and XT (b) Interaction plot for YC and XT for Layup 3, [(-45/45)2]s, loaded in tension .................................... 44 Figure 17: Runs at nominal level, with significant factors increased, and with insignificant factors increased for Layup 3, [(-45/45)2]s, loaded in tension ................ 46 Figure 18: Normal probability plot of effects for Layup 4, [(90/-45)2]s, loaded in tension ................................................................. 47 Figure 19: Normal probability plot for 27-2 factorial analysis for Layup 4, [(90/-45)2]s, loaded in tension ................................................... 48 Figure 20: Runs at nominal level, with significant factors increased, and with insignificant factors increased for Layup 4, [(90/-45)2]s, loaded in tension ................ 50 Figure 21: Interaction plot for YT and SL for Layup 4, [(90/-45)2]s, loaded in tension . 51 Figure 22: Normal probability plot of effects for Layup 5, [908], loaded in tension ... 52 Figure 23: Runs at nominal level, with significant factors increased, and with insignificant factors increased for Layup 5, [908], loaded in tension .................. 53 Figure 24: Typical loading of out-of-plane bending specimen .................................... 55 Figure 25: Normal probability plot of effects for Layup 1, [08], loaded in out-of-plane bending ....................................................... 56 Figure 26: Normal probability plot for 27-2 factorial analysis for Layup 1, [08], loaded in out-of-plane bending.......................................... 57 TABLE OF FIGURES (continued) Page Figure 27: Shear stress plots for (a) Layup 1 with SL at +20% all else at nominal level (b) Layup 3 with SL at +20% (c) Layup 1 with SL at -20% (d) Layup 3 with SL at -20% ........................................... 59 Figure 28: Runs at nominal level, with positive significant factors increased, with negative significant factor increased, with positive factors increased and negative factors decreased, and with insignificant factors increased for Layup 1, [08], loaded in out-of-plane bending ........................... 61 Figure 29: Interaction plot for XT and XC for Layup 1, [08]s, loaded in out-of-plane bending ............................................................ 62 Figure 30: Normal probability plot of effects for Layup 2, [(0/45)2]s, loaded in out-of-plane bending .................................................... 63 Figure 31: Normal probability plot for 25-1 factorial analysis for Layup 2, [(0/45)2]s, loaded in out-of-plane bending............................................... 64 Figure 32: Runs at nominal level, with significant factors increased, and with insignificant factors increased for Layup 2, [(0/45)2]s, loaded in out-of-plane bending .................................................... 65 Figure 33: Interaction plot for XT and XC for Layup 2, [(0/45)2]s, loaded in out-of-plane bending .................................................... 66 Figure 34: Normal probability plot of effects for Layup 3, [(-45/45)2]s, loaded in out-of-plane bending ................................................. 67 Figure 35: Normal probability plot for reduced 26-1 factorial analysis for Layup 3, [(-45/45)2]s, loaded in out-of-plane bending ............................ 69 Figure 36: Runs at nominal level, with significant factors increased, and with insignificant factors increased for Layup 3, [(-45/45)2]s, loaded in out-of-plane bending ................................................. 70 TABLE OF TABLES Page Table 1: Layups used ................................................................................................... 21 Table 2: Elastic material properties of the lamina [33] ................................................ 22 Table 3: Strengths of the lamina (damage initiation) [33] ........................................... 22 Table 4: Fracture energies of the lamina (damage evolution) [33] .............................. 23 Table 5: Top speeds of each car and driver combination............................................. 24 Table 6: Confounding structure for 210-5 fractional factorial experiment .................... 28 Table 7: Confounding structure for 210-4 fractional factorial experiment .................... 28 Table 8: Aliased effects for Layup 1, [08], loaded in tension ...................................... 33 Table 9: 210-5 fractional factorial for tension loading scenario .................................... 80 Table 10: 210-4 fractional factorial for out-of-plane bending loading scenario ............ 81 Table 11: 23 factorial for Layups 1 and 2 loaded in tension ........................................ 83 Table 12: 26-1 fractional factorial for Layup 3 loaded in tension ................................. 83 Table 13: 27-2 fractional factorial for Layup 4 loaded in tension ................................. 84 Table 14: 27-2 fractional factorial for Layup 1 loaded in out-of-plane bending ........... 85 Table 15: 25-1 fractional factorial for Layup 2 loaded in out-of-plane bending ........... 86 Table 16: Maximum load in pounds for 210-5 fractional factorial for tension loading scenario........................................................... 88 TABLE OF TABLES (continued) Page Table 17: Maximum moment per unit width in inch-pounds per inch for 210-4 fractional factorial for out-of-plane bending loading scenario ....................... 89 Table 18: Maximum Loads and moments per unit width in pounds and inch-pounds per inch for all additional runs in tension and then in out-of-plane bending ......................................................... 91 Table 19: Aliased effects for 23 analysis of Layup 1, [08], loaded in tension .............. 93 Table 20: Aliased effects for Layup 2, [(0/45)2]s, loaded in tension ............................ 93 Table 21: Aliased effects for 23 analysis of Layup 2, [(0/45)2]s, loaded in tension .......................................................................... 93 Table 22: Aliased effects for Layup 3, [(-45/45)2]s, loaded in tension ........................ 94 Table 23: Aliased effects for 26-1 analysis of Layup 3, [(-45/45)2]s, loaded in tension ................................................................... 94 Table 24: Aliased effects for Layup 4, [(90/-45)2]s, loaded in tension ........................ 95 Table 25: Aliased effects for 27-1 analysis of Layup 4, [(90/-45)2]s, loaded in tension ................................................................... 95 Table 26: Aliased effects for Layup 5, [908], loaded in tension .................................. 96 Table 27: Aliased effects for Layup 1, [08], loaded in out-of-plane bending .............. 96 Table 28: Aliased effects for 27-2 analysis of Layup 1, [08], loaded in out-of-plane bending ......................................................... 97 Table 29: Aliased effects for Layup 2, [(0/45)2]s, loaded in out-of-plane bending ................................................................... 97 TABLE OF TABLES (continued) Page Table 30: Aliased effects for 25-1 analysis of Layup 2, [(0/45)2]s, loaded in out-of-plane bending .................................................... 98 Table 31: Aliased effects for Layup 3, [(-45/45)2]s, loaded in out-of-plane bending ................................................................ 98 Table 32: Aliased effects for re-analysis as a 26-1 of Layup 3, [(-45/45)2]s, loaded in out-of-plane bending ................................................. 99 1 1.0 Introduction Carbon-fiber reinforced polymer (CFRP) is a material that has become more popular in aircraft design in the last few decades, and is often subjected to varying loading situations. In the unending quest to make aircraft lighter and stronger, designers have had to turn away from the use of lightweight aluminum alloys in favor of even lighter CFRP’s [1]. These composite materials are used to replace various components of an aircraft ranging from the frame [1] to the skin of the fuselage [2]. One area of concern in the design of aircraft is the stresses that occur around a cutout or a notch [3]. Often, panels, such as the fuselage of an aircraft, are loaded in tension and in out-of-plane bending [4] in the vicinity of stiffening members in the frame [5]. To properly understand the phenomena that occur near notches when a CFRP panel is subjected to tension or out-of-plane bending, Finite Element Analysis (FEA) is used. A knowledge of how panels will react and carry loads helps to ensure that the aircraft are not overdesigned, and thus heavier and more expensive. 1.1 Numerical Modeling of Composites When modeling how CFRP reacts to different loading scenarios, it is important to accurately model failure with the correct methods throughout a simulation. While elastic loading of CFRP can be modeled using classic methods of stress and strain, the elastic model is no longer valid after the specimen reaches its yield stress and damage begins through small-scale fiber breakage, matrix cracking, or fiber-matrix shearing. Just as metals and other isotropic materials can be modeled with FEA by taking into 2 account plasticity and strain hardening, composite materials can also be modeled after the elastic behavior has passed. There are several methods to model this behavior, but they all fall under the common group of progressive damage modeling [6]. Progressive damage modeling is a method of determining how damage will propagate and affect the overall strength of a CFRP laminate. Within a laminate, there are several individual layers that fail at different times and in different ways, due to the fact that they are often oriented in different directions, exposing each layer to different stresses. By using progressive damage modeling, one can determine how and when these individual lamina failures will culminate in the total failure of the entire laminate [7]. Until total failure occurs, progressive damage modeling is used to model the degradation of the strength of the laminate. Progressive damage modeling does not take into account other factors such as fatigue and manufacturing impurities causing decreased strength, but does give an accurate model disregarding these other issues. There are many different methods of modeling the progressive damage of fibrous composites such as CFRP. París [6] and Nahas [8] review over one hundred papers related to developing many of these methods. One way to classify the many different failure criteria is by whether or not the set of criteria uses specific failure modes, such as tension in the direction of the fibers, or compression in the transverse direction. The alternative to this is for the damage criteria to only identify when damage will occur within the laminate, rather than what type of damage. For example, some methods that do not have associated failure modes are Tsai-Hill [9], and TsaiWu [10]. Many more criteria do have associated failure modes, such as Hashin [11], 3 Hashin and Rotem [12], Yamada and Sun [13], and many others [14, 15, 16, 17]. These failure modes include tension and compression in the fiber direction, tension and compression in the transverse direction, matrix cracking, and fiber-matrix shearing. In papers by Hashin [11] and Hashin and Rotem [12], a method for modeling failure is developed where damage can be found in the fibers or in the matrix in either tension or compression. Chang and Chang [16] present a damage model for notched composite laminates. For their model, damage can occur not only in matrix cracking and fiber breakage, but also in fiber-matrix shearing. Shahid and Chang [17] developed another model of progressive damage that uses matrix cracking, fiber breakage, and fiber-matrix shearing. However, in Shahid and Chang’s model, Chang and Chang’s previous work and Hashin and Rotem’s work are combined to give a more comprehensive damage model. Another popular method of progressive damage modeling was developed before Hashin and Rotem developed their method, by Tsai and Wu [10]. The Tsai-Wu failure criterion, as it is named, is very broad in its applications because it can be adapted for many different materials with different symmetries and multi-axial stresses. Each of these progressive damage models requires that several material properties be obtained to fully define the criteria. Generally, the more complex a failure criterion is, the larger the number of material properties is needed. Shahid and Chang’s failure model is fairly complex, since it allows for some of the material properties to be defined as a function of crack density, rather than as a constant. Shahid and Chang argue that the first type of damage that a CFRP laminate will 4 encounter is matrix cracking, and their determination of the other failure modes depends on how much cracking has occurred. Since it is so complex, it is not practical to use Shahid and Chang’s failure criteria in most standard finite element packages. The damage criteria developed by Hashin and Rotem requires only fiber strengths, matrix strengths, shear strengths, and fracture toughnesses. Regardless of the model, the associated material properties typically need to be determined experimentally. There are several different progressive damage models, and depending on the model, two to over fourteen material properties must be known. When testing for these properties, each must be found independently, requiring many different types of tests. For the results of each type of test to be considered accurate, a minimum of five different samples must be tested [18]. With sometimes up to seventy tests that must be completed, each using a different test specimen, and several test apparatuses, a large amount of time and money can be necessary to define all of these material properties with great certainty. Testing for material properties can be a very difficult process, given the different tests and the results produced by each. The American Society for Testing and Materials (ASTM) produces standards for how to preform tests that are used to determine material properties. To test for many of the tensile material properties, one must follow ASTM standard D3039, which calls for specific specimen geometries and loading fixtures [18]. Another type of test that is necessary is a compressive test, which could be completed using ASTM standard D3410 [19], or D6641 [20]. These are only a few of the many different tests that must be performed to find the necessary 5 material properties to define a set of progressive damage criteria. The number and cost of performing all of these tests brings up the desire to know which of the material properties really affect a model of a CFRP panel. If several of these material properties have little or no effect when varied by a significant amount, then it would be reasonable to spend less time and money on getting accurate testing results by performing fewer tests. With several different material properties that are rather difficult to measure, and are generally not provided by manufacturers, it is helpful to know which of these properties will have little effect if they are not extremely accurate, and which properties will have a great effect on the outcome of a simulation. One such way to find which of these material properties are insignificant is to perform a sensitivity study [21, 22, 23]. 1.2 Sensitivity Studies A sensitivity study is a type of analysis that seeks to find how the outcome of an event can be attributed to different causes. Preforming sensitivity studies generally involves completing several simulations or physical experiments while varying levels of different factors in specific ways and comparing the level of the output. By observing the changes in the output based on the changes in the inputs, one can determine the effect of individual factors and which have more or less influence on the outcome. There are several different ways that the factors can be varied. There are two main types of sensitivity studies that can be performed based on what type of information one wishes to find: single factor variation and factorial analysis. Of the two types, the most basic type involves varying single factors 6 individually while each of the other factors remains at a constant level. For each run, the factor that is being varied can be varied at as many levels as desired to understand the effect of that factor. There are generally not many runs necessary to complete this type of study, since only one factor is being changed at a time, meaning that the number of runs is the sum of the number of levels for each factor. Using all of the runs, the results can be compared to see how much the outcome is changed by each factor. The other method that can be used is a factorial design [21, 22, 23]. The purpose of a factorial design is to compare factors to see how several factors, or combinations of factors, will affect a final outcome. In this method, each factor is varied concurrently. Usually factors are usually varied two to four levels each. The amounts of runs necessary for this method can expand rapidly, as a full factorial analysis of this type will require the product of the number of levels for each factor. For example, an analysis with five factors, varied at three levels each will require 35, or 243 runs. This type of analysis can be done with a mixed number of levels as well, meaning that one could decide that two of those factors need to be varied at only two levels. This would result in 22×33, or 108 runs. All of these runs can be combined and analyzed to provide information about each factor’s effect, as well as the effect of several factors changing at the same time. 1.3 Literature Review Sensitivity studies have been performed to determine the significance of material properties and other types of factors and how they affect results using a variety of different methods. Each study uses one of the two methods described in the 7 previous section, although some have additional variations. The following is a summary of several studies that use sensitivity studies involving material properties. A study performed by Panagiotopoulou et al. [24] examined the effects on strain values of changing properties of the periodontal ligament (PDL) while modeling mandibles of macaques. This study used the single factor variation method with different amounts of levels while using the finite element package VoxFE. The factors used were the Young’s modulus of the ligament, and the geometry of the ligament. In their study, the seven different values of Young’s modulus used for modeling the PDL were found in literature, as well as the four different geometries. Overall, a total of 12 different scenarios were run, and compared to experimental data to both validate the model, and test for the sensitivity of changing the two parameters. It was determined that the most accurate Young’s modulus for the PDL was 0.07 MPa. This value was then used to test the sensitivity of the four different geometries of the PDL. The results of those four runs were compared to modeling with no PDL, and compared to experimental data to find the best geometry. Hyer and Lee [25] performed a study on graphite composites to examine how a variational ply layup could increase the buckling load of a panel with a center-hole. This study used the finite element method varying one factor at a time. The parameters in this study were the fiber orientation in each of 18 different regions. The authors sought to optimize a layup for buckling strength using a curvilinear fiber format. Each region was varied from -90° to 90° to produce a sensitivity curve. This assumes that the best layup for each region is independent of the other regions, which they reasoned 8 to be not completely true, so a method called gradient-search [26] allowed them to find an optimized layup using all of the regions. Queiroz, Vellasco, and Nethercot [27, 28] performed a sensitivity study as part of their larger study on modeling steel-concrete composite beams for construction. This study used single factor variation for modeling the beams using ANSYS. In their study, there were three factors, the compressive strength of the concrete, the yield stress of the steel used in the web and flanges, and the ratio of strains at strain hardening and at yield. Since the sensitivity study is only a small portion of the entire study on finite element modeling, the methods used are not detailed. However, it was determined that while the strength of the concrete did have the potential to change the failure mode from slab crushing to stud failure, its effect was not as great as changing the yield stress of the web. Also, the ratio of strains at strain hardening and yield was determined to not have an effect on the response of the beam. Dar et al. [29] determine how five different factors affect the simulated stress in a cantilevered beam. This study used several different factorial analysis designs being simulated with the finite element program ANSYS. The five factors studied are the applied force, and the breadth, height, Young’s modulus, and Poisson’s ratio of the beam. In their paper, Dar et al. gave a good description of what factorial analysis is. They mentioned that a full factorial of five factors at two levels, consisting of 32 runs, was performed first. Also, they mentioned a three-level fractional factorial design using 18 runs. A fractional factorial means that not all of the effects of interactions between factors can be specifically known, as they are confounded with other effects. 9 Lastly, they actually described and developed the results of a four-level fractional factorial design that only used 16 runs. Their final design only allowed for analysis of the main factors, not interactions. They found that of the five factors, the Young’s modulus and Poisson’s ratio had no effect, and the breadth very little effect, while the other two greatly affected the measured stress. Ng, Teo, and Lee [30] conducted a factorial analysis focusing on a model of the C4-C6 vertebrae. This study used a factorial analysis while being simulated using finite element analysis. They completed a full factorial analysis of the Young’s modulus of six different portions of the model by varying each parameter ±20% in every combination available. This meant that there were 64 runs for each of three loading conditions. For each run, biomechanical responses and stresses were recorded and analyzed. It was determined that the material properties of the disc annulus had the greatest impact on both the external responses and internal stresses. This article used the most classical type two-factor factorial analysis out of the others mentioned. 1.4 Topic of this Work In this study, a sensitivity study is performed on modeling notched CFRP panels using progressive damage modeling on different ply layups under tension and out-of-plane bending to identify significant material properties. The model of progressive damage that will be used is the Hashin damage criteria. Not only is Hashin accurate and a widely used progressive damage model, but it is fully supported by the commercial FEA package Abaqus, which will be used throughout this study. These methods allow for one to differentiate in what way a laminate will fail: either in 10 tension or compression in the fiber direction, or tension or compression in the transverse direction. To fully define this set of damage criteria, these ten different material properties are necessary: Tensile and compressive strength in the fiber direction, Tensile and compressive strength in the transverse direction, Longitudinal shear strength, transverse shear strength, Tensile and compressive fracture energy for the fiber, Tensile and compressive fracture energy for the matrix. These values all appear, in one form or another, in Section 2.2, which defines the damage model for this work. The main purpose of this study is to better understand which material properties are most significant in a variety of situations. Currently, there are no studies of this kind in the literature that provide researchers with the information to know which material properties are significant to the results of a simulation. To find this information, eight fractional factorial analyses will be performed with ten factors each. The ten factors will be the ten damage parameters listed previously. There will be five different ply layups studied in in-plane tension, with three of those also being studied in out-of-plane bending. The results of this study will provide researchers with the information necessary to know which damage parameters will be most significant, and therefore, which to focus their time and money on getting more accurate values. The rest of this work will contain several sections related to the study. First, a detailed description of the progressive damage model used for this work will be given. 11 Then, the methods of the study will be discussed, including descriptions of the finite element model and the factorial analysis to be used for the sensitivity study. Following the methods will be the results and a description of what they mean for each layup being analyzed. Lastly, a comparison of the two loading scenarios will be made, and conclusions will be given regarding which damage parameters can be considered significant in the situations addressed in this work. 2.0 Progressive Damage Model 2.1 Hashin Damage Initiation In the Hashin progressive damage model, the point at which damage initiates is determined by measuring when each of several damage criteria is met. Each damage criteria compares the different measured stresses against the strength properties of the respective material. For all of the equations in the two sections, the 1-coordinate direction is aligned with the fibers, while the 2-direction coordinate is transverse to the fibers. The equations relating the modes of failure to the material properties are as follows [31]: Fiber tension ( ˆ 1 1 0 ): 2 2 ˆ ˆ t F f 1T1 1 L2 1 X S (1) 12 Fiber compression ( ˆ 1 1 0 ): ˆ c F f 1C1 X Matrix tension ( ˆ 2 2 0 2 1 (2) ): 2 t Fm Matrix compression ( ˆ 2 2 ˆ ˆ 2T2 1 L2 Y S 0 2 1 (3) ): 2 2 Y C ˆ ˆ ˆ1 2 22 2 2T 1 C L 1 T 2S S 2 S Y 2 c Fm In equations (1) through (4), ˆ i i (4) is the effective stress in the i-direction and ˆ1 2 is the effective in-plane shear stress. In the equations above, XT and XC respectively represent the tensile and compressive strengths in the direction of the fiber. Also, YT and YC respectively represent the tensile and compressive strengths in the transverse direction. Lastly, SL and ST represent the longitudinal and transverse shear strength. In equation (1), the variable α determines the contribution of shear stress to the fiber tension mode of failure, which Hashin [11] suggests should be unity. 2.2 Abaqus Energy-Based Damage Evolution Along with knowledge of how a specimen will start to fail, a loading scenario can only be fully understood if there is also knowledge of what will happen after 13 damage initiates. The commercial FEA program Abaqus employs an energy-based method which is much more complex than Hashin’s damage initiation criteria [32]. The complexity arises because rather than just finding when the linearly elastic material will start to damage, the damage evolution parameters model how the material will respond after damage has already occurred. This response is called strain softening, meaning that as the strain increases, the load carrying ability decreases. The response is computed using C d , where ε is the strain and Cd is the damaged elasticity matrix, as shown in equation (5). Cd (1 d f ) (1 d m ) (1 d f ) E 1 1 (1 d f ) (1 d m ) 1 2 E 2 D 0 (1 d m ) E 2 0 21 E1 0 (1 d s ) G D 0 (5) In this equation, D is a combination of variables as shown in equation (6), while df, dm, and ds are damage state variables for the fiber, matrix, and shear, respectively. E1, E2, G, ν12, and ν21 are the usual orthotropic elastic constants. D 1 (1 d f )(1 d m ) 1 2 2 1 (6) Each of the three damage state variables is derived from damage variables that correspond to the four damage initiation modes. The three equations corresponding to damage states are as follows: d f d d t f c f dm dm c dm t if ˆ 1 1 0 if ˆ 1 1 0 if ˆ 2 2 0 if ˆ 2 2 0 (7) (8) 14 d s 1 (1 d f )(1 d f )(1 d m )(1 d m ) t c t c (9) In equations (7) and (8), ˆ 1 1 and ˆ 2 2 have the same definitions as in equations (1) through (4). Information is gathered from the loading profile of the material and used to define what the damage variables are. Abaqus has rid the functions which involve the damage variables of mesh dependency by using a characteristic length so that the constitutive law can be in terms of stress and displacement, rather than stress and strain. A simplified depiction of what the stress-displacement plot looks like using Abaqus’ damage evolution is shown in Figure 1. Figure 1: Equivalent stress versus equivalent displacement (adapted from [32]) 15 When damage has been initiated in a particular mode, the equivalent stress-equivalent displacement relationship, shown in Figure 1, controls how the material properties will degrade. The equivalent displacement and equivalent stress for each of the modes can be calculated as follows: Fiber tension ( ˆ 1 1 0 ): eq L ft Fiber compression ( ˆ 1 1 11 ft eq 0 2 (10) c (11) 11 (12) eq L ft ): fc 0 12 11 12 12 eq L Matrix tension ( ˆ 2 2 2 11 c fc eq c 11 eq fc 11 L (13) c ): eq L mt mt eq c 22 22 2 12 2 22 12 12 eq mt L c (14) (15) 16 Matrix compression ( ˆ 2 2 0 ): eq L mc eq mc 2 22 c 12 (16) 2 22 12 12 22 eq mc L (17) c In equations (10) through (17), Lc is the characteristic length of the element, which is defined as the square root of the area for shell elements. Also in equations (10) through (17), the bracket symbols represent the Macaulay bracket operator, which is defined in equation (18) for any variable, x. x x x (18) 2 Using the equivalent stress-equivalent displacement relationship, after the point where damage occurs, which can be represented as e q eq 0 in Figure 1, the damage variable for each mode can be calculated using equation (19). eq eq eq f d 0 eq eq eq f 0 (19) This damage variable varies from 0 at the point damage initiates to 1 at the point labeled e fq in Figure 1. The piece of information that is missing from this method is the area under the equivalent stress-equivalent displacement profile, which is known as the fracture energy, Gc [32]. Since the slope of the left side of the profile can be calculated from the Young’s modulus, and the height of the profile is the equivalent strength, the area 17 under the curve is all that is necessary to determine the full profile, and thus the damage variables. To properly define damage evolution for a material, this Gc value must be known for each of the failure modes. 3.0 Methods The methods of this study can be broken down into two main sections; finite element modeling, and factorial analysis. The modeling for this study consists of a finite-element model of a notched CFRP panel subjected to boundary conditions that represent in-plane tension and out-of-plane bending. The factorial analysis that was used is a fractional factorial analysis using either a 210-4 or 210-5 construction, depending on whether the analysis was for bending or tension, respectively. 3.1 Finite Element Model The finite element model used in this study is a conventional shell model using Abaqus’ S4 element with four nodes. This type of element provides accurate modeling without greatly increasing the computational time needed for each run. Each element consists three integration points through the thickness for each lamina. The mesh, which is fine near the notch where damage is most common and coarse near the edges, can be seen in Figure 2. 18 Figure 2: Mesh of finite element model This mesh is particularly suited for this study because of its high density of equal sized elements surrounding the notch. With increasingly small elements near the notch tip, an unrealistic concentration of stress and damage tends to occur, so keeping elements that are approximately equal in size around the notch is important. The size of the smaller elements around the notch tip was chosen because this mesh was the coarsest mesh that showed convergence with an elastic solution. That is, when modeled without damage, this mesh was the coarsest that did not significantly alter the results. Coarser meshes provide different results, while finer meshes do not have a significant effect. The entire model is made up of 3868 elements that are approximately 0.0625 inches on a side near the notch, and 0.25 inches by 0.5 inches on the outer edges of the model. The two different loading scenarios that are used for the study have different boundary conditions which are shown in Figure 3 and Figure 4. 19 Figure 3: Boundary conditions for specimen loaded in tension Figure 4: Boundary conditions for specimen loaded in bending 20 The FEA models for the specimen loaded in bending are based on previous studies performed by Kennedy et al. [5] and Arias [33]. In their study, Kennedy et al. were able to accurately model physical experiments with the device shown in Figure 5 using the methods used in this study to within ten percent. Their work validates the model, and its ability to accurately simulate the loading conditions used for this study. Figure 5: Physical bending apparatus for proprietary testing [5] 21 In order to have results that can be applied to many different situations, five different symmetric ply layups are used, as shown in Table 1. These layups consist of eight plies, each 0.006 inches thick, arranged symmetrically, each using a combination of 0°, 90°, 45°, and -45° fiber orientations. Table 1: Layups used Layup 1 Layup 2 Layup 3 Layup 4 Layup 5 0° 0° -45° 90° 90° 0° 45° 45° -45° 90° 0° 0° -45° 90° 90° 0° 45° 45° -45° 90° 0° 45° 45° -45° 90° 0° 0° -45° 90° 90° 0° 45° 45° -45° 90° 0° 0° -45° 90° 90° For this study, a CFRP material that is fully described in a study by Wong et al. [34] is used. In Table 2 through Table 4, all of the nominal material properties are given for this material. Table 2 lists the elastic properties for the CRFP lamina, Table 3 lists all the strength properties that are needed to define the Hashin damage initiation criteria, and Table 4 lists the fracture energies needed for the Abaqus specified damage evolution criteria. 22 Table 2: Elastic material properties of the lamina [34] Material Property Value E1 (psi) 1.91E+07 E2 (psi) 1.38E+06 ν12 0.326 G12 (psi) 7.64E+05 G13 (psi) 1.02E+06 G23 (psi) 4.92E+05 Table 3: Strengths of the lamina (damage initiation) [34] Damage Parameter Factor Label Nominal Value XT (psi) A 1.93E+05 XC (psi) B 1.57E+05 YT (psi) C 1.03E+04 YC (psi) D 3.21E+04 SL (psi) E 1.03E+04 ST (psi) F 1.37E+04 23 Table 4: Fracture energies of the lamina (damage evolution) [34] Damage Parameter Factor Label Nominal Value Gft (lb/in) G 11.42 Gfc (lb/in) H 11.42 Gmt (lb/in) I 1.88 Gmc (lb/in) J 1.88 3.2 Factorial Analysis For this work, a two-level fraction factorial analysis was used. In a two-level factorial analysis, each of the factors is given a high and a low value, which represent the two levels. Each of the runs will produce a result that can then be compared to the other results using a specific method, as defined in the section to follow. A symbolic example using two different cars and two different drivers will help illustrate a two factor analysis. In Table 5, the top speeds for each driver, labeled A, are paired with each car, labeled B. There are two different types of effects that can be estimated from this data; the main effect, and the interaction effect. Both of these types of effects can be better explained by considering another type of effect, the simple effect. The simple effect contrasts the two values for one factor, while holding the other factor constant. For example, the simple effect of the car type (factor A in Table 5) on the top speed with the first driver (factor B1) is the difference between the two speeds, or 65 – 68 = -3. Similarly, the simple effect of factor A with the second 24 driver is 97 – 60, or 37. The main effect of each factor is the average of the simple effects for that factor. For example, the main effect of factor A is the average of 37 and -3, or 17, while the main effect of factor B is the average of -8 and 32, or 12. Lastly, the interaction effect is the difference between the simple effects of one factor at two different levels of another factor. For example, the interaction effect of factor B with factor A is defined as the difference between 37 and -3, or the difference between 32 and -8, which has a result of 40 in both cases. This simple explanation of a factorial analysis with two factors can be greatly expanded and complicated to solve much more difficult problems. Table 5: Top speeds of each car and driver combination Driver (B) Car (A) Driver 1 (B1) Driver 2 (B2) Car Means Car 1 (A1) 68 60 64.0 Car 2 (A2) 65 97 81.0 66.5 78.5 Driver Means When dealing with more factors, a two-level factorial treatment design is made that uses high and low values for each of the factors, resulting in a 2n factorial. The reason it is referred to as a 2n factorial is that to discover all of the main effects and 25 interaction effects, there must be 2n different runs, usually found through either experimentation or simulation. By inspecting the results of the tests, one can find the simple effects of each factor at constant levels of the other factors, which leads to finding the main effect of each factor as well as the interaction effects of any two, three, and so on up to n factors. The problem with a full 2n factorial is that the amount of experiments or analyses expands rapidly with the amount of factors. The solution to this problem is to use a fractional factorial. In many situations, completing a full factorial treatment design is a large task with more experiments than one can do within a reasonable amount of time with limited resources, but the analysis produces a great deal of information. A fractional factorial requires far fewer runs, but loses resolution at the higher-order interaction levels. The information given by a full factorial treatment is so expansive, that it may not be fully necessary in providing an understanding of the situation that is being analyzed. For example, with a full 27 factorial design, a minimum of 128 runs of a process are necessary to gather the results. The results given by this type of factorial include 7 main effects, 21 two-factor interaction effects, 35 three-factor interaction effects and an additional 64 interaction effects that include four or more factors. These high-order interactions of several factors generally have a smaller effect than lowerorder interactions, and can be considered negligible. Fractional factorial experiment designs cut the amount of runs necessary in half, quarter, eighth, or even smaller fractions, depending on how much resolution one is willing to lose and how many runs are feasible. With each increasing cut of the full 26 factorial, more and more interaction factors get confounded. For example, in a 23-1 fractional factorial, only four runs are necessary, rather than the full factorial which requires eight. However, since effects are confounded, it is impossible to tell the difference between the main effect of one factor, and the interaction effect of the other two. This issue is known as aliasing or confounding. This phenomenon has less of an influence as the factorial becomes larger. For example, in a 25-1 fractional factorial, 16 runs are needed, rather than 32, and each of the main effects is aliased with only a four-factor interaction affect, which can generally be ignored. However, if fewer than half of the original runs are desired, a 2n-p factorial is necessary, where p changes how many runs will be necessary to complete the analysis. However, p must be kept relatively small, because each effect will have 2p-1 aliases. An example of a fractional factorial design that has been reduced to the point that aliasing becomes a major issue is a 27-4 fractional factorial where each main effect is aliased with three different twolevel interactions. To determine how much aliasing will occur, fractional factorial analyses can be characterized in several classes, known as the resolution of the analysis. A Resolution III factorial means that no main effects are aliased with each other, but they are aliased with two-factor interactions. In a Resolution IV factorial, all main effects are only aliased with three-factor or higher interactions, but two-factor interactions are confounded with other two-factor interactions. A Resolution V factorial has no main effect or two-factor interaction that is confounded with any other main effect or two-factor interaction. The use of the proper resolution of fractional factorial greatly reduces the amount of runs without losing too much vital information. 27 A fractional factorial can even be used to merely weed out factors that have little or no effect at all, and allow for a smaller full factorial to take place with only the factors that have larger effects. For this study, two different fractional factorial designs were used, depending on the loading scenario. The two different factorial designs are a 210-5 and a 210-4 fractional factorial design which can be found in Table 9 and Table 10 respectively, in Appendix A. In each of the designs, the two levels used are twenty percent above and twenty percent below the nominal value of the particular factor. For the tension cases, the factorial design used is a 210-5 fractional factorial design, which is Resolution III. For the bending cases, the design is a 210-4 fractional factorial design, which is Resolution IV. The confounding structure of both of these is found in Table 6 and Table 7. 28 Table 6: Confounding structure for 210-5 fractional factorial experiment Aliases LA = A+BJ LAC = AC+FG LBG =BG+CI LB =B+AJ LAD = AD+EF LBH =BH LC =C LAE = AE+DF LCD =CD+EG+HJ LD =D LAF = AF+BI+CG+GI LCE =CE+DG LE =E LAG = AG+CF LCH =CH+DJ LF =F+IJ LAH = AH LCJ =CJ+DH LG =G LAI = AI+BF LEH =EH+GJ LH =H LBC =BC+GI LEJ =EJ+GH LI =I+FJ LBD =BD+EI LFH =FH LJ =J+AB+FI LBE =BE+DI LHI =HI Table 7: Confounding structure for 210-4 fractional factorial experiment Aliases LA = A LAB = AB+GH LBD = BD LCI = CI+DJ LEJ = EJ LB = B LAC = AC LBE = BE LCJ = CJ+DI LFG = FG LC = C LAD = AD LBF = BF LDE = DE LFH = FH LD = D LAE = AE LBI = BI LDF = DF LFI = FI LE = E LAF = AF LBJ = BJ LDG = DG LFJ = FJ LF = F LAG = AG+BH LCD = CD+IJ LDH = DH LGI = GI LG = G LAH = AH+BG LCE = CE LEF = EF LGJ = GJ LH = H LAI = AI LCF = CF LEG = EG LHI = HI LI = I LAJ = AJ LCG = CG LEH = EH LHJ = HJ LJ = J LBC = BC LCH = CH LEI = EI 29 The 210-5 analysis for the tension scenarios is repeated for each of the five ply layups, while the 210-4 analysis for bending is repeated for only the first three ply layups. The resulting analysis of all the runs produces a set of significant factors, which identify which material properties have the greatest effect on maximum load in each of the different cases. The method for determining which factors are significant uses a normal probability plot. The purpose of this method is to determine whether differences in results can be attributed to random variation that would be acceptable with a normal distribution, or if they are markedly different due to changes in levels of the factors. When the effects of each factor are paired with values of a normal distribution, centered at zero, and plotted, a straight line would signify that the values fall within normal probability and that the differing levels of factors have no effect. On the contrary, if any of the plotted effects do not lie on a straight line, they cannot be labeled chance occurrences, but rather direct effects of a factor. In their text, Box, Hunter, and Hunter [35], give an example using a process development study with four factors. The normal plot is shown in Figure 6. In this plot, the points labeled LA, LD, LBD, and LB clearly do not lie on a line, as all the other factors do. In this case, it can be claimed that those four factors are significant and cause changes outside the range of normal distribution. 30 Figure 6: Normal plot example showing significant factors [34] 4.0 Results The results for this study can be broken down into separate categories, based on loading condition. The first set of results are for the in-plane tension loading scenario, while the second set of results correspond to the data gathered from the outof-plane bending runs. The method of plotting the values of effects on a normal plot is used to determine which factors are significant. For each of the layups, a normal probability plot of the effects will be given with significant effects labeled. Each of the effects will be labeled with a code that corresponds to letters assigned to each factor. 31 In cases where two letters are given, that signifies that the effect in the interaction between two factors. The reason the code is given, rather than just the factors, is due to the fact that some of the effects are confounded with other effects, so the code could correspond to two or more different sets of effects based on the confounding structures shown in Table 6 and Table 7. 4.1 In-Plane Tension Each of the five layups described in Table 1 were simulated as being loaded in tension until after the maximum load had been reached, and significant unloading had occurred due to damage and reduced load-carrying capabilities of the specimen. The reason it was necessary to ensure that significant unloading had occurred was due to the fact that in some cases, a small amount of damage can cause a drop in the load, but the specimen can still continue to hold more load with increased displacement. A typical load versus displacement plot of this scenario is shown in Figure 7. Each of the layups had a total of 32 different runs with the factors varied up or down as shown in Table 9 in Appendix A. The resulting maximum loads are recorded in Table 16 and Table 18 in Appendix B. 32 Figure 7: Typical loading of tensile specimen The first layup, consisting of eight 0° plies produced effects which are shown in order in Table 8 to show how the effects translate to a plot, and graphed with a line showing the approximate standard distribution in Figure 8. For the remaining layups, tables of the effects can be found in Appendix C. For this layup, there was only one significant effect, which was LA. 33 Table 8: Aliased effects for Layup 1, [08], loaded in tension LA LB LC LD LE LF LG LH LI LJ 3031 -622 -294 -36 198 428 463 -238 -110 -20 LAC LAD LAE LAF LAG LAH LAI LBC LBD LBE -648 -678 870 -213 586 -690 -480 38 -460 68 LBG LBH LCD LCE LCH LCJ LEH LEJ LFH LFI 245 -223 -99 -804 -90 541 -207 -534 504 -451 Figure 8: Normal probability plot of effects for Layup 1, [08], loaded in tension 34 The analysis of the results of the first layup revealed that the most significant effect in the load carrying ability of the specimen was LA. This effect corresponds to either the main factor of the tensile strength in the fiber direction, XT, or the interaction between compressive strength in the fiber direction and compressive fracture energy of the matrix, or XC and Gmc. To avoid any unnecessary assumptions, another smaller factorial analysis was performed using only the three factors that might be involved. This 23 factorial design can be found in Table 11 in Appendix A, with results in Table 18 in Appendix B. The normal probability plot for this factorial analysis is shown in Figure 9. 35 Figure 9: Normal probability plot for 23 factorial analysis for Layup 1, [08], loaded in tension The additional analysis revealed that LBJ, which was initially confounded with LA, is not significant. Therefore, since the effect LA is significant in both factorial designs, it is the significant effect. The effect LA corresponds to the main effect of factor XT for the first layup, which means that the strength of the fibers has the greatest effect on the overall strength of the laminate. In the scope of this study, these results for the first layup loaded in tension mean that a high level of accuracy is necessary for XT, while it is not necessary for the other material properties. To prove this explicitly, three additional runs were 36 completed. For the first run, each material property was set at the nominal (accurate) value as shown in Table 3 and Table 4. The next run had only XT at an increased level of 20%, with the other nine factors (XC, YT, YC, SL, ST, Gft, Gfc, Gmt, and Gmc) at the nominal level. Lastly, the nine insignificant factors were increased by 20%, while XT was left at the nominal level. The results are shown in Figure 10. This can be interpreted as showing that by increasing all of the insignificant factors, there was less of an effect on the solution than when increasing only the significant factor. When increasing only the significant factor, the result increases by 20.5%, while the result only increases by 11.6% when the other nine factors are increased at the same time. Figure 10: Runs at nominal level, with significant factors increased and others at nominal level, and with insignificant factors increased and significant factors at nominal level for Layup 1, [08], loaded in tension 37 The two different factorial analyses, as well as the individual case study all support each other and have common results. When dealing with a CFRP panel that has all 0° plies loaded in tension, the most important material property to find with a high level of accuracy is the tensile fiber strength. The second layup, which consists of 0° and 45° plies alternating, produced fairly similar results. While somewhat less defined, the effect LA is still the only significant factor for this layup as well. All of the effects for Layup 2 are plotted on a normal probability plot in Figure 11. Figure 11: Normal probability plot of effects for Layup 2, [(0/45)2]s, loaded in tension 38 The analysis of the results of the second layup revealed that again, the most significant effect in the load carrying ability of the specimen was LA. The same process of performing a second smaller factorial analysis, as described in Table 11 with resulting maximum loads in Table 18, was completed using the same 23 design as before. The normal probability plot for this factorial analysis is shown in Figure 12. Figure 12: Normal probability plot for 23 factorial analysis for Layup 2, [(0/45)2]s, loaded in tension 39 The additional analysis revealed that LBJ, which was initially confounded with LA, is not significant. Therefore, since the effect LA is significant in both factorial designs, it is the significant effect. The effect LA corresponds to the main effect of factor XT for the second layup, which means that the strength of the fibers has the greatest effect on the overall strength of the laminate. The biggest difference between the second layup and the first was the magnitude at which this effect influenced the result. Rather than contributing over 3,000 pounds to the load carrying ability in the 210-5 factorial study, the effect LA contributed merely 1,500 pounds. This is due to the fact that half of the plies were not oriented in line with the loading, and therefore, the fibers were not in as much direct tension. The same type of case study that was performed for the last layup was again performed for this one. Since the same factor was significant, the same there runs were completed with Layup 2. The results are shown in Figure 13. This can be interpreted as showing that by increasing all of the insignificant factors, the resulting maximum load decreased by 1.5%, while increasing the significant factor increased the load by 27.3%. 40 Figure 13: Runs at nominal level, with significant factors increased, and with insignificant factors increased for Layup 2, [(0/45)2]s, loaded in tension For the second layup, loaded in tension, all of the different types of analyses again agreed and had the same results. Thus, when dealing with a CFRP panel that has alternating 0° and 45° plies loaded in tension, the most important material property to find with a high level of accuracy is the tensile fiber strength. The third layup, which consists of -45° and 45° plies alternating, had a different effect that was most significant, but also had other significant effects as well. The most significant effect was LE, followed by two other significant effects; LA and LAE. All of the effects for Layup 3 plotted on a normal probability plot in Figure 14. 41 Figure 14: Normal probability plot of effects for Layup 3, [(-45/45)2]s, loaded in tension The third layup is the first time that the results and analysis do not reveal a clear-cut significant effect. The effect LE is has only one associated factor, which is the longitudinal shear strength, or SL. This factor was not a surprise due to the fact that there should be shearing forces between the plies due to the fact that the plies are perpendicular to each other. Also, the 45° angles that the plies are being pulled at would cause the plies to slide against each other as the specimen elongates. The other two significant effects are both confounded with two-factor interactions, so additional analysis was necessary. To ensure that the previous results are correct, every factor 42 that could possibly be involved was included in a 26-1 factorial analysis. This factorial design can be found in Table 12 in Appendix A, with results in Table 18 in Appendix B. The normal probability plot for this factorial analysis is shown in Figure 15. Figure 15: Normal probability plot for 26-1 factorial analysis for Layup 3, [(-45/45)2]s, loaded in tension The second factorial analysis revealed much of the same results as the first one for this layup. In this case, LE is still the most significant, followed by LAE and LA. The two confounded factors, LDF and LBJ are both insignificant in this analysis. Therefore, 43 LA corresponds to the main effect of XT and LAE corresponds to the effect of the interaction between XT and SL. Thus the significant factors, in order of significance, are the main effect of factor SL, the main effect of factor XT, and the interaction effect of factors XT and SL. This layup is the first time that an interaction between two factors has been significant, so further explanation will be provided. A method that is commonly used to visualize interaction effects is called an interaction plot, which can be generated using the program Statgraphics. In this plot, there are two lines which each track the average response of a factor at each level, which is the maximum load in this case. One line represents the response at the low level of a second factor, while the other line represents the high level of that second factor. If the lines have a large slope, then the first factor is significant on its own. If the two lines are far apart, this signifies that that second factor is significant. However, the important part of this type of plot is the differences in the slopes of the lines. If the two lines have very similar slopes, the interaction effect is insignificant. However, if the two lines have differing slopes, this signifies that the interaction will have an effect on the overall response. In other words, the effect of a factor depends on the level of another factor, whereas with an insignificant interaction, the effect of a factor is independent of the other. Using results from the 210-5 analysis for this layup, the significant interaction of SL and XT is shown in Figure 16 (a), while an insignificant interaction, XT and YC is shown in Figure 16 (b). 44 Figure 16: (a) Interaction plot for SL and XT (b) Interaction plot for YC and XT for Layup 3, [(-45/45)2]s, loaded in tension In this case, the specific interpretation of Figure 16 (a) is important to understanding the interaction effect. The dashed line shows that when SL is at a low 45 level, XT has a fairly low effect, an average of approximately 50 pounds. The solid line shows that when SL is at a high level, XT has a much higher effect of approximately 350 pounds on average. Therefore, the interaction between SL and XT is significant. A simple interpretation of Figure 16 (b) shows that no matter what the level of YC is, XT has an effect of approximately 200 pounds. Since there are multiple significant effects, the case study method that was previously used had to be altered slightly. This time, both SL and XT are significant, as well as their interaction, so for the “significant effects” run, both of these factors were increased by 20%, while the “insignificant effects” run consisted of raising the other 8 factors by 20%. The results for this case study are shown in Figure 17. In this case, increasing the significant factors caused a 26.3% increase in maximum load, while the insignificant factors increased the result by only 5.3%. 46 Figure 17: Runs at nominal level, with significant factors increased, and with insignificant factors increased for Layup 3, [(-45/45)2]s, loaded in tension All of the different analyses that were completed for this layup agreed and pointed to a common answer. When dealing with a CFRP panel that has alternating 45° and 45° plies loaded in tension, the most important material properties to find with high levels of accuracy are the longitudinal shear strength and the tensile fiber strength. This is due to the fact that both of these factors are significant, as well as their interaction. The fourth layup, which consists of 90° and -45° plies alternating, had the largest number of significant effects, but also was very clear with its insignificant effects. The most significant effect was LC, followed by three other significant effects; 47 LE, LCE and LI. All of the effects for Layup 4 are plotted on a normal probability plot in Figure 18. Figure 18: Normal probability plot of effects for Layup 4, [(90/-45)2]s, loaded in tension The analysis of the runs for the fourth layup revealed a total of four significant effects. The first two significant effects have no aliasing with any other main effects or two-factor interactions, and are therefore correlated to the transverse tensile strength 48 and the longitudinal shear strength, or YT and SL, respectively. The next two factors both have confounding issues, so again, additional analysis is necessary. This time, with all of the significant factors, there were a total of 7 different factors involved in some way. Thus, a 27-2 factorial analysis was necessary to clear up any ambiguity. This factorial design can be found in Table 13 in Appendix A, with results in Table 18 in Appendix B. The normal probability plot for this factorial analysis is shown in Figure 19. Figure 19: Normal probability plot for 27-2 factorial analysis for Layup 4, [(90/-45)2]s, loaded in tension 49 As previously stated, the effects LC and LE are both unconfounded and correspond to the main effects of YT and SL. However, the effect LCE could previously have corresponded to the interaction between YT and SL, or the interaction between YC and Gft, which are the compressive strength in the transverse direction and the tensile fracture energy of the fiber. The 27-2 factorial analysis proved that LCE corresponds to the interaction between YT and SL. The effect LI could have corresponded to the main effect of Gmt, the tensile fracture energy of the matrix, or the interaction between ST and Gmc, the transverse shear strength and the compressive fracture energy of the matrix. The 27-2 factorial analysis proved that LI corresponds to the main effect of Gmt. Thus, the four significant effects for the fourth layup are the main effect of factor YT, the main effect of factor SL, the interaction effect of factors YT and SL, and the main effect of factor Gmt. This means that the tensile strength of the laminate in the transverse direction, as well as the shear strength in the direction of the fibers, their interaction, and the tensile fracture energy of the matrix are most likely to have an effect on the overall strength of the laminate. For this layup, the case study consisted of a run with nominal values for each factor, a run with YT, SL, and Gmt increased by 20% and the other factors at nominal level, and a run with all of the insignificant factors increased by 20% while the significant factors are held at the nominal level. The results of these three runs are shown in Figure 20. This shows that increasing the significant factors by 20% increases the resulting maximum load by 19.4%, while increasing the insignificant factors has no effect at all on the result. 50 Figure 20: Runs at nominal level, with significant factors increased, and with insignificant factors increased for Layup 4, [(90/-45)2]s, loaded in tension Since one of the significant effects is an interaction between two factors, an interaction plot from Statgraphics is useful to get a better understanding of what is happening. In Figure 21, the dashed line represents the average of the runs where YT is at a low level, and the effect of SL is only about 25 pounds. However, when YT is at a high level, as represented by the solid line, the effect of SL is approximately 160 pounds. Therefore, the effect of SL is dependent on the level of YT, and vice versa. 51 Figure 21: Interaction plot for YT and SL for Layup 4, [(90/-45)2]s, loaded in tension Again, the four different types of analyses support the same results and conclusions. When dealing with a CFRP panel that has alternating 90° and -45° plies loaded in tension, the most important material properties to find with high levels of accuracy are the tensile strength in the transverse direction, the longitudinal shear strength, and the tensile fracture energy of the matrix. This is due to the fact that each of these factors are significant, as well as the interaction between two of them. The fifth and final layup, which consists of eight 90° plies, had only one significant effect. The most significant effect was LC. All of the effects for Layup 5 are plotted on a normal probability plot in Figure 22. 52 Figure 22: Normal probability plot of effects for Layup 5, [908], loaded in tension The fifth and final layup produced the clearest significant factor out of all of the layups. This is not only due to the fact that the plot of the normal probability revealed a very clear outlier, but also due to the fact that the effect had no confounded two-factor interaction effects. The effect LC only corresponds to one factor, which is the tensile strength in the transverse direction, YT. Much like the first layup that contained only 0° plies and had a significant factor that was the tensile strength of the fibers, this layup contains only 90° plies, which directly leads to a significant factor that is the tensile strength in the transverse direction. 53 For the fifth layup, the same type of case study was performed with the single significant factor being compared to the other nine insignificant factors. The results are shown in Figure 23. The effect of increasing the single significant factor by 20% was an increase in maximum load of 19.4%. However, increasing the other nine insignificant factors by 20% only resulted in increasing the maximum load by 0.2%. With this, it is clear that the single significant effect is important to find with high accuracy, while the others do not have a very large effect. Figure 23: Runs at nominal level, with significant factors increased, and with insignificant factors increased for Layup 5, [908], loaded in tension The results of the case study match with the original factorial analysis, and therefore, the results were confirmed. When dealing with a CFRP panel that has all 54 90° plies loaded in tension, the most important material property to find with a high level of accuracy is the tensile strength in the transverse direction, while the other properties will have a lesser effect on the maximum load carrying ability of the panel. 4.2 Out-of-Plane Bending Three layups, Layup 1 through Layup 3 as described in Table 1, were loaded in out-of-plane bending. Only three layups are analyzed for the bending loading scenario is that the specimen does not respond well with the last two layups due to their compliant nature. The last two layups failed to reach maximum loads in almost all values of material properties. The specimens were deflected to their maximum allowable value, and still continued to bend but not break. For the three layups that were modeled, a 210-4 fractional factorial was performed, allowing for less aliasing and a clearer set of significant effects. Since there are fewer factors that are confounded, as shown in Table 7, there are 49 different main factor and two-factor interactions that create effects, rather than 30 in the previous 210-5 analysis. The load versus displacement plot for a typical bending run, as shown in Figure 24, has a similar shape to that of the tension scenario, however, the amplitude is typically much less, and the load is measured as a moment per unit width. The runs that were performed involved changing each factor by twenty percent above or below as dictated by the plan shown in Table 10, located in Appendix A. The resulting calculated maximum moments per unit width are recorded in Table 17 in Appendix B. For each of the three layups the normal probability plot will be given. 55 Figure 24: Typical loading of out-of-plane bending specimen The first layup, consisting of eight 0° plies produced four significant effects which are labeled in Figure 25. There were three positive effects, LA, LB, and LAB. There were also four negative effects, LE, LAE, LBE, and LCJ. 56 Figure 25: Normal probability plot of effects for Layup 1, [08], loaded in out-of-plane bending Since this analysis was done on a 210-4 fractional factorial, there is far less confounding of the effects, but with so many factors that are significant, an additional 27-2 factorial analysis was necessary. This factorial design can be found in Table 14 in Appendix A, with results in Table 18 in Appendix B. The normal probability plot for this factorial analysis is shown in Figure 26. 57 Figure 26: Normal probability plot for 27-2 factorial analysis for Layup 1, [08], loaded in out-of-plane bending The results of this analysis clear up any previous concerns about confounding, as well as showing that some of the effects that were previously thought to be significant are actually insignificant. With the new 27-2 factorial analysis the significant effects are LA, LB, LAB, and LE, the last of which is a negative effect. These effects correspond to the main effects of XT, XC, their interaction effect, and the main effect of SL. The interesting thing about the analysis for this layup is not necessarily which effects are significant, but how they are significant. This is the first layup thus far in the analysis that produced a negatively significant factor. 58 Normally, an effect that is positive means that an increase in the factor causes an increase in the result; or a decrease in the factor causes a decrease in the result. However, in the case of a negatively significant effect, an increase in the factor causes a decrease in the result, while a decrease in the factor causes an increase in the result. In this particular scenario, since the factor in question is the longitudinal shear strength, this means that increased shear strength will cause a decrease in load carrying ability. While this can be confusing on the surface, that an increase in a particular strength will decrease overall strength, it can be explained. When the individual laminas are all facing the 0°-direction and have increased shear strength, it causes a sort of embrittlement of the overall laminate. The laminas cannot flex and bend against each other very easily. If a specimen with high shear strength is loaded in bending, it will be more likely to break at areas of high stress, which are the places near the notch tips with fewer loads being applied. However when the shear strength is lower, there is a little bit more compliance between the individual laminates, which allows the complete laminate to flex more before it breaks and carry more load. To illustrate this, the shear stress can be used to show this phenomenon, since SL is the longitudinal shear strength. Additional runs were performed varying only SL by 20% above and below the nominal level with the first and third layups, loaded in out-ofplane bending. For these four runs, plots were produced using Abaqus to show the shear stress at the point of maximum applied moment. In Figure 27 (a), a stress concentration can be seen near the notch tip which caused the premature breakage of the panel, even with a higher strength. In Figure 27 (b) through (d), the shear stress 59 does not show any concentrations that would cause the behavior previously seen. The stress concentration and premature failure only appear in the model which had higher shear strength when that parameter had a negative significance. Figure 27: Shear stress plots for (a) Layup 1 with SL at +20% all else at nominal level (b) Layup 3 with SL at +20% (c) Layup 1 with SL at -20% (d) Layup 3 with SL at -20% 60 To better illustrate the phenomenon of a negative effect, the normal case study was altered to show the effect. This time, there were five runs completed in the case study. The first run consisted of all ten factors at their nominal level. Next, a run was completed with XT and XC increased by 20% and the other eight factors at their nominal levels. Then, a run was completed with only SL increased by 20%. This was followed by a run that had XT and XC increased by 20% and SL decreased by 20% to give a run that would provide the maximum possible result using only the significant factors. Lastly, a run with the seven factors not involved in the previous two runs being increased by 20% was completed. The results of this case study are shown in Figure 28. By increasing the seven insignificant factors by 20%, the resulting maximum moment decreased by 7.2 %. This can be compared to increasing SL, the negative effect, by 20%, which resulted in a decrease of 29.8%, and an increase in XT and XC, which increased the result by 11.8%, and an increase in XT and XC coupled with a decrease in SL, which increased the result by 69.5%. 61 Figure 28: Runs at nominal level, with positive significant factors increased, with negative significant factor increased, with positive factors increased and negative factors decreased, and with insignificant factors increased for Layup 1, [08], loaded in out-of-plane bending This layup has an interaction effect as one of the significant effects, so additional support from an interaction plot will help to clarify how this effect acts. In Figure 29, the dashed line represents the average of the runs where XT is at a low level, and the effect of XC is only about 13 inch-pounds per inch. However, when XT is at a high level, as represented by the solid line, the effect of XC is approximately 71 inchpounds per inch. Therefore, the effect of XC is dependent on the level of XT, and vice versa. 62 Figure 29: Interaction plot for XT and XC for Layup 1, [08]s, loaded in out-of-plane bending Therefore, the four significant effects for the first layup loaded in out-of-plane bending, as supported by all of the presented analysis methods, are the main effect of factor XT, the main effect of factor XC, the interaction effect of factors XT and XC, and the main effect of factor SL. The second layup, which consists of 0° and 45° plies alternating, produced similar results. The clear significant effects, in order of significance are LA, LB, and LAB. All of the effects for Layup 2 are plotted on a normal probability plot in Figure 30. 63 Figure 30: Normal probability plot of effects for Layup 2, [(0/45)2]s, loaded in out-ofplane bending The analysis second layup, consisting of 0° and 45° plies produced fairly clearcut results. The three significant effects revealed for this layup were LA, LB, and LAB. While LA and LB are both unconfounded and correspond to only one effect, the interaction effect LAB could correspond to two different effects, which required additional analysis. To clear up the confounding, a 25-1 factorial analysis was performed using the four factors that may have been involved, as well as SL, to provide additional factors to compare to without a significant increase in necessary runs. This fractional factorial design and its results can be found in Table 15 and Table 18, 64 respectively. The normal probability plot for this factorial analysis is shown in Figure 31. Figure 31: Normal probability plot for 25-1 factorial analysis for Layup 2, [(0/45)2]s, loaded in out-of-plane bending The results of the additional factorial analysis prove that the effect LAB corresponds to the interaction between XT and XC rather than the interaction between Gft and Gfc. Thus, the three significant effects for the second layup, loaded in out-ofplane bending are the main effect of the factor XT, the main effect of the factor XC, and 65 the interaction effect of the factors XT and XC. As with the other layups, a case study of three runs was completed. The three runs used nominal levels, significant factors increased by 20%, and insignificant factors increased by 20%. The results are shown in Figure 32. By increasing the factors included in the significant effects by 20%, the resulting maximum moment increases by 25.7%. However, increasing the eight insignificant factors by 20% only increases the maximum moment by 1.4%. Figure 32: Runs at nominal level, with significant factors increased, and with insignificant factors increased for Layup 2, [(0/45)2]s, loaded in out-of-plane bending This layup also has an interaction effect as one of the significant effects, so additional support from an interaction plot will help to clarify how this effect acts. In Figure 33, the dashed line represents the average of the runs where XT is at a low level, 66 and the effect of XC is only about 3 inch-pounds per inch. However, when XT is at a high level, as represented by the solid line, the effect of XC is approximately 27 inchpounds per inch. Therefore, the effect of XC is dependent on the level of XT, and vice versa. Figure 33: Interaction plot for XT and XC for Layup 2, [(0/45)2]s, loaded in out-of-plane bending The results of the four different analyses produced the same results, and are thus conclusive. Only the tensile and compressive strengths in the fiber direction will have a significant effect on the results. This can be interpreted in the focus of this study to mean that it is important to accurately measure the tensile and compressive strengths in the fiber direction when analyzing a CFRP panel consisting of alternating 0° and 45° plies, while other damage parameters are much less crucial. 67 The third layup, which consists of -45° and 45° plies alternating, had the most difficult effect structure to analyze. The aliased effects are plotted on a normal probability plot in Figure 34. There are three effects which are clearly significant; LE, LA, and LB, but there are many more that are on the border of being considered significant or insignificant. The ambiguous effects, in order, are as follows: LAE, LAB, LBE, LEJ, LCJ, LG, LAJ, and LAC. Figure 34: Normal probability plot of effects for Layup 3, [(-45/45)2]s, loaded in outof-plane bending 68 For this layup loaded in out-of-plane bending, the results were much more convoluted and required further analysis. The three effects that were clearly significant are ones that are common to other two layups as well, LE, LA, and LB. As previously mentioned, these effects correspond to the main effects of the factors SL, XT, and XC. After that the analysis becomes more difficult. There are eight additional effects that are ambiguous as to whether they are significant or not. However, when looking at the eleven total effects that have varying levels of significance, only six factors are involved. At this point, four of the factors can be eliminated, leaving two replications of a 26-1 factorial design. No additional runs were necessary to create this new factorial design, the original results were used, but the effects that were clearly insignificant were eliminated from the analysis. The analysis for this design is very much the same as the analysis for the original 210-4 design, only with fewer factors. The normal probability plot for this new analysis is shown in Figure 35. 69 Figure 35: Normal probability plot for reduced 26-1 factorial analysis for Layup 3, [(45/45)2]s, loaded in out-of-plane bending For this new normal probability plot, it is pretty clear that using only the factors that may have contributed to a significant effect, the only truly significant effects are LE, LA, and LB. These three effects correspond to the main effects of the factors SL, XT, and XC, respectively. To show this explicitly, another case study was performed with SL, XT, and XC increased by 20% with the other factors at nominal level. The results for this study are shown in Figure 36. This shows that an increase of 20% in the significant factors creates an increase in the maximum moment of 26.8%, 70 while an equivalent increase in the insignificant factors increases the maximum moment by only 5.5%. Figure 36: Runs at nominal level, with significant factors increased, and with insignificant factors increased for Layup 3, [(-45/45)2]s, loaded in out-of-plane bending From the preceding analyses, the shear strength in the direction of the fibers, as well as the tensile and compressive strengths of the fibers will have a noticeable effect on the results, while the other factors will not. Therefore, it is crucial to determine these values to a higher level of accuracy, while the insignificant damage parameters can be off by as much as 20% without significantly altering the resulting model. 71 5.0 Discussion For the first three layups that were analyzed, the specimens were modeled in both in-plane tension and out-of-plane bending. This allows some comparisons between the two types of loading scenarios, allowing for generalization of the results. Each of the three layups that were loaded in both scenarios did not have the exact same significant effects for the two loading scenarios, but there were similarities. The first layup showed slightly different results when modeled in tension and in out-of-plane bending. There was one extremely significant effect when loaded in tension, which was the main effect of XT. However, when the specimen was modeled in out-of-plane bending, there were three significant effects; the main effect of XT was still the most significant, but others were added in as well. Since in-plane tension produces a fairly even field of loading throughout the specimen, it is expected that tensile strength is an important factor. Conversely, bending the specimen produces tension on the outside of the curved part, and compression on the inside. This explains why the bending analysis revealed that the compressive strength in the fiber direction was significant. Also, the interface between plies, as each ply has differing levels of tension and compression on opposite sides, creates an importance for the shear strength of the material, which explains why the main effect of the factor SL is significant. The second layup produced very similar, but slightly less extreme, results when compared to the first layup. This is most likely due to the fact that in both 72 bending and tension, these ply layups gain most of their strength from the fibers. In cases where the load is not uniaxial or the bending is not about a single axis, it is more necessary to have fibers going in multiple directions to increase the versatility of the material. However, since the specimen modeled with the second layup is only loaded uniaxially, and bent about one axis, the strength of the fibers in the direction of the load tends to wash out other properties. This explains why the significant factors for the second layup are so similar to those of the first layup. The third layup does not have any 0° plies to dominate the load carrying ability of the specimen, and therefore, another factor rises to the top as the most significant. In both tension and out-of-plane bending, the longitudinal shear strength becomes the most significant factor, but the tensile strength in the direction of the fibers is still important, being the second most significant factor. As described previously, the specimens loaded in tension experience only tension, while the specimens loaded in bending experience both bending and compression of the CFRP throughout the thickness of the lamina. This explains why the compressive strength in the direction of the fibers also appears as a significant factor when analyzing the out-of-plane bending scenario. In the frame of this study, several thoughts can be considered regarding the necessity of testing for material properties. When tasked with finding material properties, it is evident from the eight cases discussed in this study that not all ten of the damage parameters have the same effect of the outcome of modeling CFRP panels 73 in tension and out-of-plane bending. For layups that have a significant number of zerodegree plies, the strengths in the direction of the fibers are material properties that merit spending extra time and money to ensure a more accurate number, and thus, a more accurate model. When a specimen is loaded in tension, only the tensile strengths are important, but when the loading scenario is out-of-plane bending, the panel experiences both tension and compression, which means that both strength parameters need to be known with a higher level of accuracy. When there are few or no zerodegree plies, other material properties become more important to know with significantly higher accuracy. For example, if the layup for a specimen is dominated by ninety-degree plies, it would be wise to spend more time and money getting an accurate value for the transverse strength, rather than the strength in the fiber direction. In every case in this study that had an interaction as a significant effect, the two factors involved in the interaction were also significant. Thus when testing for damage parameters, if those the two parameters involved in an interaction are known at a high level of accuracy, the interaction between those effects will not cause the model to have deficiencies. It was rare for one of the fracture energies to be considered significant, so in most cases, those energies do not need to be known with a high level of accuracy to maintain an accurate model. 6.0 Conclusion The use of CFRP panels and other structures has grown significantly in the last few decades as manufacturing processes and technology have expanded and become 74 more efficient. One area that has not kept up with the use of CFRP is the ability for engineers to properly and accurately model different scenarios where this lightweight, strong material might be used. A specific field where this applies greatly is the aerospace industry, which is trending away from using bulky metals in favor of the sleeker alternative, CFRP. In the aerospace industry, a common use for CFRP panels is as the skin of the fuselage of aircraft. When used in this application, these panels experience loading in tension and in bending, so knowledge of how to properly model both scenarios is necessary. Progressive damage modeling has been in existence for well over forty years, but there are still problems with its utility in modeling CFRP’s. For one, depending on the method of modeling used, there can be well over ten to fifteen damage parameters that are necessary to determine when and how a CFRP panel will fail. These damage parameters are costly and difficult to obtain, so an understanding of which parameters will have the greatest effect on accurate modeling is greatly desired. With this knowledge, extra time and money can be spent on those significant parameters, while others can be regarded with less importance to the overall accuracy of the model. The results of this study provided very valuable information for the specific cases presented, but the methods may be even more valuable, especially in cases that are dissimilar to those presented here. If a specific layup or loading scenario is to be modeled and material properties are not known, the methods of this study can be applied to determine where resources should be focused when finding them. Using 75 generic material properties, such as those found in Wong et al. [34], performing a factorial analysis to determine which material properties are significant will take far less time and resources than actually finding each of the ten properties at a high level of accuracy. Often, only two or three of the properties will be significant and require additional testing, while the others can continue to be modeled using those generic properties. Performing an analysis similar to the ones presented in this study can provide far more valuable information than doing several material property tests for values that have little or no effect on a model, even when they are off by as much as twenty percent. 76 7.0 Bibliography [1] H. M. Flower and C. Soutis, "Materials for airframes," Aeronautical Journal, vol. 107, no. 1072, pp. 331-341, 2003. [2] P. Linde, A. Schulz and W. Rust, "Influence of modelling and solution methods on the FE-simulation of the post-buckling behaviour of stiffened aircraft fuselage panels," Composite Structures, vol. 73, no. 2, pp. 229-236, 2006. [3] D. R. Ambur, N. Jaunky and M. W. Hilburger, "Progressive failure studies of stiffened panels subjected to shear loading," Composite Structures, vol. 65, pp. 129-142, 2004. [4] C. B. Prasad, M. J. Shuart, N. J. Bains and M. Rouse, "Effects of cutouts on the behavior of symmetric composite laminates subjected to bending and twisting loads," NASA Report N95-28844, 1995. [5] T. C. Kennedy, J. P. Parmigiani, S. A. Gonzalez and T. J. Luedeman, "Failure of notched laminates under out-of-plane bending," Air Traffic Organization Report DOT/FAA/AR-xx/xx, 2010. [6] F. París, "A Study of Failure Criteria of Fibrous Composite Materials," NASA Report CR-2001-210661, 2001. [7] R. M. Christensen, "Failure of fiber composite laminates - Progressive damage and polynomial invariants," 8 August 2009. [Online]. Available: http://www.failurecriteria.com/Media/Failure_of_Fiber_Composite_Laminates_Progressive_Damage_and_Polynomial_Invariants.pdf. [Accessed 12 August 2012]. [8] M. N. Nahas, "Survey of Failure and Post-Failure Theories of Laminated FiberReinforced Composites," Journal of Composites Technology & Research, vol. 8, no. 4, pp. 138-153, 1986. [9] V. D. Azzi and S. W. Tsai, "Anisotropic Strength of Composites," Experimental Mechanics, vol. 5, no. 9, pp. 283-288, 1965. 77 [10] S. W. Tsai and E. M. Wu, "A general theory of strength for anisotropic materials," Journal of Composite Materials, vol. 5, pp. 58-80, 1971. [11] Z. Hashin, "Failure Criteria for Unidirectional Fiber Composites," Journal of Applied Mechanics, vol. 47, no. 1, pp. 329-334, 1980. [12] Z. Hashin and A. Rotem, "A Fatigue Criterion for Fiber-Reinforced Materials," Journal of Composite Materials, vol. 7, pp. 448-464, 1973. [13] S. E. Yamada and C. T. Sun, "Analysis of Laminate Strength and its Distribution," Journal of Composite Materials, vol. 12, pp. 275-284, 1978. [14] L. J. Hart-Smith, "A New Approach to Fibrous Composite Laminate Strength Prediction," in Eighth DOD/NASA/FAA Conference on Fibrous Composites in Structural Design, NASA CP-3208, pp. 663-693, 1989. [15] A. Puck and W. Schneider, "On Failure Mechanisms and Filure Criteria of Filament-Wound Glass/Resin Composites," Plastics and Polymers, vol. 37, pp. 33-43, 1969. [16] F.-K. Chang and K.-Y. Chang, "A Progressive Damage Model for Laminated Composites Containing Stress Concentrations," Journal of Composite Materials, vol. 21, no. 9, pp. 934-855, 1987. [17] I. Shahid and F.-K. Chang, "An Accumulative Damage Model for Tensile and Shear Failures of Laminated Composite Plates," Journal of Composite Materials, vol. 29, no. 7, pp. 926-981, 1995. [18] "Standard Test Method for Tensile Properties of Polymer Matrix Composite Materials," ASTM Standard D3039/D3039M-08, 2010. [19] "Standard Test Method for Compressive Properties of Polymer Matrix Composite Materials with Unsupported Gage Section by Shear Loading," ASTM Standard D3410/D3410M-03(2008), 2010. [20] "Standard Test Method for Compressive Properties of Polymer Matrix Composite Materials Using a Combined Loading Compression (CLC) Test Fixture," ASTM Standard D6641/D6641M-09, 2010. 78 [21] R. O. K uehl, Design of Experiments: Statistical Principles of Research Design and Analysis, Pacific Grove, CA: Duxbury/Thomson Learning, 2000. [22] D. C. Montgomery, Design and Analysis of Experiments, Hoboken, NJ: John Wiley & Sons, 2005. [23] D. C. Montgomery, G. C. Runger and N. F. Hubele, "Design of Engineering Experiments," in Engineering Statistics, Hoboken, NJ, John Wiley & Sons, 2007, pp. 341-413. [24] O. Panagiotopoulou, K. Kupczik and S. N. Cobb, "The mechanical function of the periodontal ligament in the macaque mandible: a validation and sensitivity study using finite element analysis," Journal of Anatomy, vol. 218, no. 1, pp. 7586, 2011. [25] M. W. Hyer and H. H. Lee, "The use of curvilinear fiber format to improve buckling resistance of composite plates with central circular holes," Composite Structures, 1991. [26] H. Miura and L. A. Schmit, "NEWSUMT: A Fortran program for inequality constrained function minimization: Users guide," NASA CR-159070, 1979. [27] F. D. Queiroz, P. G. Vellasco and D. A. Nethercot, "Finite element modelling of composite beams with full and partial shear connection," Journal of Constructional Steel Research, vol. 63, no. 4, pp. 505-521, 2007. [28] F. D. Queiroz, P. G. Vellasco and D. A. Nethercot, "Finite element modelling of steel-concrete composite beams subjected to uniform loads," in The tenth international conference on civil, structural and environmental engineering computing, 2005. [29] F. H. Dar, J. R. Meakin and R. M. Aspden, "Statistical methods in finite element analysis," Journal of Biomechanics, vol. 35, pp. 1155-1161, 2002. [30] H. W. Ng, E. C. Teo and V. S. Lee, "Statistical factorial analysis on the material property sensitivity of the mechanical responses of the C4-C6 under compression, anterior and posterior shear," Journal of Biomechanics, vol. 37, pp. 771-777, 2004. 79 [31] "Damage initiation for fiber-reinforced composites," in Abaqus 6.11 Analysis User's Manual, Providence, RI, Dassault Systèmes, 2011. [32] "Damage evolution and element removal for fiber-reinforced composites," in Abaqus 6.11 Analysis User's Manual, Providence, RI, Dassault Systèmes, 2011. [33] S. G. Arias, "Failure Analysis of Pre-notched Composite Laminated Plates under Four-point Bending Conditions," Doctor of Philosophy, Mechanical Engineering, Oregon State University, Corvallis, OR, 2009. [34] K. J. Wong, X. J. Gong, S. Aivazzadeh and M. N. Tamin, "Tensile behaviour of anti-symmetric CFRP composite," Procedia Engineering, vol. 10, pp. 1865-1870, 2011. [35] G. E. Box, J. S. Hunter and W. G. Hunter, Statistics for Experimenters: Design, Innovation, and Discovery, Hoboken, New Jersey: John WIley & Sons, Inc., 2005. 80 Appendix A: Fractional Factorial Designs Table 9: 210-5 fractional factorial for tension loading scenario Run 1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 XT -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 XC -1 -1 1 1 -1 -1 1 1 -1 -1 1 1 -1 -1 1 1 -1 -1 1 1 -1 -1 1 1 -1 -1 1 1 YT -1 -1 -1 -1 1 1 1 1 -1 -1 -1 -1 1 1 1 1 -1 -1 -1 -1 1 1 1 1 -1 -1 -1 -1 YC -1 -1 -1 -1 -1 -1 -1 -1 1 1 1 1 1 1 1 1 -1 -1 -1 -1 -1 -1 -1 -1 1 1 1 1 SL 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 ST 1 -1 1 -1 1 -1 1 -1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 1 -1 1 -1 Gft 1 1 1 1 -1 -1 -1 -1 -1 -1 -1 -1 1 1 1 1 -1 -1 -1 -1 1 1 1 1 1 1 1 1 Gfc 1 -1 -1 1 -1 1 1 -1 -1 1 1 -1 1 -1 -1 1 1 -1 -1 1 -1 1 1 -1 -1 1 1 -1 Gmt 1 1 -1 -1 1 1 -1 -1 -1 -1 1 1 -1 -1 1 1 -1 -1 1 1 -1 -1 1 1 1 1 -1 -1 Gmc 1 -1 -1 1 1 -1 -1 1 1 -1 -1 1 1 -1 -1 1 1 -1 -1 1 1 -1 -1 1 1 -1 -1 1 81 29 30 31 32 -1 1 -1 1 -1 -1 1 1 1 1 1 1 1 1 1 1 -1 -1 -1 -1 1 -1 1 -1 -1 -1 -1 -1 1 -1 -1 1 1 1 -1 -1 1 -1 -1 1 Table 10: 210-4 fractional factorial for out-of-plane bending loading scenario Run 1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 XT -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 XC -1 -1 1 1 -1 -1 1 1 -1 -1 1 1 -1 -1 1 1 -1 -1 1 1 -1 -1 1 1 -1 -1 YT -1 -1 -1 -1 1 1 1 1 -1 -1 -1 -1 1 1 1 1 -1 -1 -1 -1 1 1 1 1 -1 -1 YC -1 -1 -1 -1 -1 -1 -1 -1 1 1 1 1 1 1 1 1 -1 -1 -1 -1 -1 -1 -1 -1 1 1 SL -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 1 1 1 1 1 1 1 1 1 1 ST -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 Gft 1 1 -1 -1 -1 -1 1 1 -1 -1 1 1 1 1 -1 -1 1 1 -1 -1 -1 -1 1 1 -1 -1 Gfc 1 -1 1 -1 -1 1 -1 1 -1 1 -1 1 1 -1 1 -1 1 -1 1 -1 -1 1 -1 1 -1 1 Gmt 1 -1 -1 1 1 -1 -1 1 -1 1 1 -1 -1 1 1 -1 -1 1 1 -1 -1 1 1 -1 1 -1 Gmc 1 -1 -1 1 -1 1 1 -1 1 -1 -1 1 -1 1 1 -1 -1 1 1 -1 1 -1 -1 1 -1 1 82 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 1 1 -1 -1 1 1 -1 -1 1 1 -1 -1 1 1 -1 -1 1 1 -1 -1 1 1 -1 -1 1 1 -1 -1 1 1 -1 -1 1 1 -1 -1 1 1 1 1 -1 -1 -1 -1 1 1 1 1 -1 -1 -1 -1 1 1 1 1 -1 -1 -1 -1 1 1 1 1 -1 -1 -1 -1 1 1 1 1 1 1 -1 -1 -1 -1 -1 -1 -1 -1 1 1 1 1 1 1 1 1 -1 -1 -1 -1 -1 -1 -1 -1 1 1 1 1 1 1 1 1 1 1 -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 1 1 1 1 1 1 1 1 1 1 1 1 -1 -1 -1 -1 -1 -1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 -1 -1 -1 -1 1 1 1 1 -1 -1 1 1 -1 -1 -1 -1 1 1 -1 -1 1 1 1 1 -1 -1 1 1 -1 -1 -1 1 1 -1 1 -1 -1 1 -1 1 1 -1 1 -1 1 -1 1 -1 -1 1 -1 1 -1 1 -1 1 1 -1 1 -1 1 -1 1 -1 -1 1 1 -1 -1 1 1 -1 -1 1 1 -1 -1 1 -1 1 1 -1 -1 1 1 -1 -1 1 1 -1 -1 1 1 -1 1 -1 -1 1 1 -1 1 -1 -1 1 1 -1 -1 1 -1 1 1 -1 1 -1 -1 1 -1 1 1 -1 -1 1 1 -1 1 -1 -1 1 -1 1 1 -1 83 61 62 63 64 -1 1 -1 1 -1 -1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 -1 -1 1 1 -1 1 -1 1 1 -1 -1 1 1 -1 -1 1 Gft × × × × × × × × Gfc × × × × × × × × Gmt × × × × × × × × Gmc 1 -1 1 -1 1 -1 1 -1 Gfc × × × × × × × × × × × × × Gmt × × × × × × × × × × × × × Gmc -1 1 1 -1 1 -1 -1 1 1 -1 -1 1 -1 Table 11: 23 factorial for Layups 1 and 2 loaded in tension Run 1 2 3 4 5 6 7 8 XT 1 1 1 1 -1 -1 -1 -1 XC 1 1 -1 -1 1 1 -1 -1 YT × × × × × × × × YC × × × × × × × × SL × × × × × × × × ST × × × × × × × × Table 12: 26-1 fractional factorial for Layup 3 loaded in tension Run 1 2 3 4 5 6 7 8 9 10 11 12 13 XT -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 XC -1 -1 1 1 -1 -1 1 1 -1 -1 1 1 -1 YT × × × × × × × × × × × × × YC -1 -1 -1 -1 1 1 1 1 -1 -1 -1 -1 1 SL -1 -1 -1 -1 -1 -1 -1 -1 1 1 1 1 1 SC -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 Gft × × × × × × × × × × × × × 84 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 1 -1 -1 1 1 -1 -1 1 1 -1 -1 1 1 -1 -1 1 1 × × × × × × × × × × × × × × × × × × × 1 1 1 -1 -1 -1 -1 1 1 1 1 -1 -1 -1 -1 1 1 1 1 1 1 1 -1 -1 -1 -1 -1 -1 -1 -1 1 1 1 1 1 1 1 1 -1 -1 -1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × 1 1 -1 1 -1 -1 1 -1 1 1 -1 -1 1 1 -1 1 -1 -1 1 Gfc × × × × × × × × × × × Gmt 1 -1 -1 1 -1 1 1 -1 -1 1 1 Gmc 1 -1 -1 1 1 -1 -1 1 -1 1 1 Table 13: 27-2 fractional factorial for Layup 4 loaded in tension Run 1 2 3 4 5 6 7 8 9 10 11 XT × × × × × × × × × × × XC × × × × × × × × × × × YT -1 1 -1 1 -1 1 -1 1 -1 1 -1 YC -1 -1 1 1 -1 -1 1 1 -1 -1 1 SL -1 -1 -1 -1 1 1 1 1 -1 -1 -1 ST -1 -1 -1 -1 -1 -1 -1 -1 1 1 1 Gft -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 -1 85 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × × 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 1 -1 -1 1 1 -1 -1 1 1 -1 -1 1 1 -1 -1 1 1 -1 -1 1 1 -1 1 1 1 1 -1 -1 -1 -1 1 1 1 1 -1 -1 -1 -1 1 1 1 1 1 1 1 1 1 -1 -1 -1 -1 -1 -1 -1 -1 1 1 1 1 1 1 1 1 -1 -1 -1 -1 -1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 × × × × × × × × × × × × × × × × × × × × × -1 1 -1 -1 1 1 -1 -1 1 -1 1 1 -1 -1 1 1 -1 1 -1 -1 1 -1 -1 1 1 -1 -1 1 1 -1 -1 1 1 -1 1 -1 -1 1 1 -1 -1 1 Table 14: 27-2 fractional factorial for Layup 1 loaded in out-of-plane bending Run 1 2 3 4 5 6 7 8 9 XT -1 1 -1 1 -1 1 -1 1 -1 XC -1 -1 1 1 -1 -1 1 1 -1 YT -1 -1 -1 -1 1 1 1 1 -1 YC × × × × × × × × × SL -1 -1 -1 -1 -1 -1 -1 -1 1 ST × × × × × × × × × Gft -1 -1 -1 -1 -1 -1 -1 -1 -1 Gfc 1 -1 -1 1 -1 1 1 -1 -1 Gmt × × × × × × × × × Gmc 1 -1 -1 1 1 -1 -1 1 -1 86 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 -1 1 1 -1 -1 1 1 -1 -1 1 1 -1 -1 1 1 -1 -1 1 1 -1 -1 1 1 -1 -1 -1 1 1 1 1 -1 -1 -1 -1 1 1 1 1 -1 -1 -1 -1 1 1 1 1 × × × × × × × × × × × × × × × × × × × × × × × 1 1 1 1 1 1 1 -1 -1 -1 -1 -1 -1 -1 -1 1 1 1 1 1 1 1 1 × × × × × × × × × × × × × × × × × × × × × × × -1 -1 -1 -1 -1 -1 -1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 -1 1 -1 -1 1 1 -1 -1 1 -1 1 1 -1 -1 1 1 -1 1 -1 -1 1 × × × × × × × × × × × × × × × × × × × × × × × 1 1 -1 -1 1 1 -1 -1 1 1 -1 -1 1 1 -1 1 -1 -1 1 1 -1 -1 1 Table 15: 25-1 fractional factorial for Layup 2 loaded in out-of-plane bending Run 1 2 3 4 5 6 7 XT -1 1 -1 1 -1 1 -1 XC -1 -1 1 1 -1 -1 1 YT × × × × × × × YC × × × × × × × SL -1 -1 -1 -1 1 1 1 ST × × × × × × × Gft -1 -1 -1 -1 -1 -1 -1 Gfc 1 -1 -1 1 -1 1 1 Gmt × × × × × × × Gmc × × × × × × × 87 8 9 10 11 12 13 14 15 16 1 -1 1 -1 1 -1 1 -1 1 1 -1 -1 1 1 -1 -1 1 1 × × × × × × × × × × × × × × × × × × 1 -1 -1 -1 -1 1 1 1 1 × × × × × × × × × -1 1 1 1 1 1 1 1 1 -1 -1 1 1 -1 1 -1 -1 1 × × × × × × × × × × × × × × × × × × 88 Appendix B: Results for Each Factorial Analysis Table 16: Maximum load in pounds for 210-5 fractional factorial for tension loading scenario Run 1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 Layup 1 5760 12342 5760 10401 5759 7445 5759 9451 5759 11366 5759 8926 5761 9702 5761 7650 5742 8841 5380 7588 6303 9487 5737 10310 6613 8280 6579 9034 9477 Layup 2 6314 5978 3628 6214 3836 7623 3836 5343 3623 5736 3724 5548 3841 5341 3837 5349 5928 6276 3597 5455 3389 5241 3389 5212 3621 5174 5999 4942 3369 Layup 3 2721 2977 2723 2965 2460 2944 2412 2802 2638 2863 2844 2870 2378 2922 2350 2874 1952 2106 1995 2177 2219 2153 2270 2188 2178 2187 2157 2117 1979 Layup 4 896.5 896.5 866.9 866.9 1255 1255 1251 1251 866.9 866.9 896.5 896.5 1250 1251 1255 1255 837 837 870.3 870.3 1082 1082 1100 1100 870.3 870.3 837 837 1100 Layup 5 573.7 573.7 566.5 566.5 843.6 843.6 843.1 843.1 566.5 566.5 573.7 573.7 843 843.1 843.6 843.6 564.9 564.9 570.7 570.7 837.5 837.5 837.6 837.6 570.7 570.7 564.9 564.9 837.6 89 30 31 32 8113 5623 7086 4885 3369 5176 2063 1906 2109 1100 1082 1082 837.6 837.5 837.5 Table 17: Maximum moment per unit width in inch-pounds per inch for 210-4 fractional factorial for out-of-plane bending loading scenario Run 1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 Layup 1 109.586 140.528 115.028 249.170 82.795 161.268 123.786 265.483 105.634 123.291 120.758 269.806 92.690 133.045 121.231 264.120 78.030 111.824 85.518 136.771 84.320 107.347 89.680 147.737 84.092 101.107 Layup 2 70.917 81.473 69.169 122.075 67.721 81.873 68.454 102.413 68.308 82.318 71.356 121.050 70.160 81.021 66.491 109.314 70.976 82.638 71.977 103.438 69.73 84.164 81.255 103.976 68.995 87.120 Layup 3 49.746 54.414 55.160 60.078 488.875 53.142 50.819 60.975 46.661 54.553 57.658 60.500 50.514 55.355 50.187 61.144 57.861 62.456 57.703 73.500 54.021 63.023 59.785 76.663 52.750 63.724 90 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60 89.371 138.303 78.030 104.635 86.978 132.697 102.845 151.532 121.392 266.451 108.281 155.245 118.607 266.957 120.363 122.117 117.093 260.730 94.432 151.346 124.806 150.113 84.360 100.941 87.894 139.805 77.996 104.549 86.978 142.759 78.030 104.88 91.498 135.13 73.849 108.682 69.825 83.542 72.552 106.043 68.032 82.135 71.597 123.441 70.390 79.917 65.862 104.877 70.255 80.694 69.201 122.635 68.308 81.460 69.042 108.113 69.445 84.843 80.048 106.614 69.815 82.2363 78.819 102.196 70.796 83.638 69.027 112.842 64.205 74.760 55.549 61.461 59.309 76.380 46.987 53.757 55.865 59.760 50.902 53.368 43.322 59.388 48.188 55.082 56.323 58.944 49.052 53.827 51.305 59.955 52.362 64.218 63.427 74.677 55.121 60.903 59.158 75.713 55.075 61.267 60.547 74.280 91 61 62 63 64 84.320 107.957 89.68 156.09 69.773 85.556 80.581 103.602 53.707 62.831 59.400 77.607 Table 18: Maximum Loads and moments per unit width in pounds and inch-pounds per inch for all additional runs in tension and then in out-of-plane bending Run 1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 Layup 1 9776 9290 9438 9078 6242 6242 7367 7205 Layup 2 5799 5906 5695 6351 3657 3657 3783 3783 Layup 3 2226 2174 2226 2174 2226 2174 2226 2174 2518 2995 2518 2995 2486 3051 2486 3053 2226 2185 2226 2173 2226 2163 2226 2163 2486 Layup 4 870.3 1082 837 1100 866.9 1255 896.5 1251 837 1100 870.3 1082 896.5 1251 866.9 1255 870.3 1082 837 1100 866.9 1255 896.5 1251 837 Layup 1 106.479 123.964 130.687 166.683 93.558 147.515 119.047 264.473 84.165 101.139 88.4478 135.901 76.492 100.750 82.492 146.397 128.283 118.585 146.324 266.829 95.623 160.771 100.618 195.823 77.475 Layup 2 69.232 79.531 66.411 110.184 69.423 86.070 71.808 102.899 68.979 82.412 69.012 103.505 71.109 83.074 80.360 104.136 92 26 27 28 29 30 31 32 2995 2486 2995 2518 2995 2518 2995 1100 870.3 1082 896.5 1251 866.9 1255 102.225 86.406 140.116 77.996 104.67 89.680 147.603 93 Appendix C: Calculated Effects for Each Analysis Table 19: Aliased effects for 23 analysis of Layup 1, [08], loaded in tension LA LB LJ LAB LAJ LBJ LABJ 2632 -385 252 660 171 -9 72 Table 20: Aliased effects for Layup 2, [(0/45)2]s, loaded in tension LA LB LC LD LE LF LG LH LI LJ 1512 -347 -545 -483 297 92 9 621 -61 -30 LAC LAD LAE LAF LAG LAH LAI LBC LBD LBE 401 -166 300 -239 -333 -316 180 96 642 -254 LBG LBH LCD LCE LCH LCJ LEH LEJ LFH LFI 306 -163 145 325 -295 -221 66 75 -63 -136 Table 21: Aliased effects for 23 analysis of Layup 2, [(0/45)2]s, loaded in tension LA LB LJ LAB LAJ LBJ LABJ 2218 -148 -191 -22 -191 137 137 94 Table 22: Aliased effects for Layup 3, [(-45/45)2]s, loaded in tension LA LB LC LD LE LF LG LH LI LJ 195 1 -90 39 624 -7 78 29 42 -16 LAC LAD LAE LAF LAG LAH LAI LBC LBD LBE 65 2 140 7 -23 -2 -10 -27 2 -10 LBG LBH LCD LCE LCH LCJ LEH LEJ LFH LFI -13 77 -70 -92 -3 15 2 -26 -31 86 Table 23: Aliased effects for 26-1 analysis of Layup 3, [(-45/45)2]s, loaded in tension LA LB LD LE LF LJ LAB LAD LAE LAF 226.9 -0.6 5.1 556.4 -7.9 -0.9 -0.6 5.1 280.4 -7.9 LAJ LBD LBE LBF LBJ LDE LDF LDJ LEF LEJ -0.9 0.9 0.9 -0.9 -13.1 9.1 -1.1 0.6 -6.4 0.6 LFJ -0.6 95 Table 24: Aliased effects for Layup 4, [(90/-45)2]s, loaded in tension LA LB LC LD LE LF LG LH LI LJ 0.1 0.1 304.3 -0.1 95.0 0.1 -0.1 -0.1 21.3 -0.1 LAC LAD LAE LAF LAG LAH LAI LBC LBD LBE 0.1 0.1 0.1 -0.1 0.1 -2.5 -0.1 0.1 -4.4 0.1 LBG LBH LCD LCE LCH LCJ LEH LEJ LFH LFI -10 0.1 -0.1 66.9 -0.1 -0.1 -0.1 -0.1 0.1 0.1 Table 25: Aliased effects for 27-1 analysis of Layup 4, [(90/-45)2]s, loaded in tension LC LD LE LF LG LI LJ LCD LCE LCF 304.3 0 95.0 0 0 21.2 0 0 67.0 0 LCG LCI LCJ LDE LDF LDG LDI LDJ LEF LEG 0 -10.2 0 0 -2.6 0 0 0 0 0 LEI LEJ LFG LFI LFJ -4.4 0 0 0 0 96 Table 26: Aliased effects for Layup 5, [908], loaded in tension LA LB LC LD LE LF LG LH LI LJ 0 0 271.5 0 4.0 0 0 0 3.4 0 LAC LAD LAE LAF LAG LAH LAI LBC LBD LBE 0 0 0 0 0 -0.2 0 0 0.5 0 LBG LBH LCD LCE LCH LCJ LEH LEJ LFH LFI -3.1 0 0 1.7 0 0 0 0 0 0 Table 27: Aliased effects for Layup 1, [08], loaded in out-of-plane bending LA LB LC LD LE LF LG LH LI LJ 70.0 50.5 5.1 -5.6 -43.5 5.8 -9.7 -9.4 -6.9 9.2 LAB LAC LAD LAE LAF LAG LAH LAI LAJ LBC 34.3 4.6 -10.4 -20.5 -0.2 -9.0 -5.8 -2.7 7.9 1.1 LBD LBE LBF LBI LBJ LCD LCE LCF LCG LCH -4.3 -18.0 -0.8 1.7 5.2 -7.4 8.1 1.1 -7.7 -5.9 LCI LCJ LDE LDF LDG LDH LEF LEG LEH LEI 1.0 -12.5 1.2 -5.8 -0.7 0.5 6.2 0.1 -1.9 -4.5 LEJ LFG LFH LFI LFJ LGI LGJ LHI LHJ -3.5 -7.7 -6.0 0.3 7.5 9.1 0.7 8.7 0.6 97 Table 28: Aliased effects for 27-2 analysis of Layup 1, [08], loaded in out-of-plane bending LA LB LC LE LG LH LJ LAB LAC LAE 52.5 38.0 0 -45.2 4.4 2.4 -3.8 25.0 14.1 -13.0 LAG LAH LAJ LBC LBE LBG LBH LBJ LCE LCG 1.8 4.4 0.9 -1.9 -14.0 0.5 -10.4 -0.5 1.3 -11.7 LCH LCJ LEG LEH LEJ -8.7 10.4 -3.1 -1.0 2.5 Table 29: Aliased effects for Layup 2, [(0/45)2]s, loaded in out-of-plane bending LA LB LC LD LE LF LG LH LI LJ 25.4 15.1 -2.5 0.4 0.6 0.4 0.8 -0.4 0.5 0.6 LAB LAC LAD LAE LAF LAG LAH LAI LAJ LBC 12.2 -2.8 1.4 -3.3 -0.2 -2.1 0.9 -0.5 2.5 -2.1 LBD LBE LBF LBI LBJ LCD LCE LCF LCG LCH 0.1 -1.2 0.6 0.9 0.6 0.3 2.4 -0.3 -0.2 -0.2 LCI LCJ LDE LDF LDG LDH LEF LEG LEH LEI -0.6 -4.4 -0.2 -0.1 -0.4 -0.5 0.3 0.2 -0.4 1.0 LEJ LFG LFH LFI LFJ LGI LGJ LHI LHJ -2.6 0.2 0 0.4 -0.5 -0.3 0.1 -0.2 0 98 Table 30: Aliased effects for 25-1 analysis of Layup 2, [(0/45)2]s, loaded in out-of-plane bending LA LB LE LG LH LAB LAE LAG LAH LBE 23.2 12.3 2.5 0.9 1.2 10.1 -2.3 -2.3 2.2 0.1 LBG LBH LEG LEH LGH 0.5 -0.7 1.2 -1.9 -3.5 Table 31: Aliased effects for Layup 3, [(-45/45)2]s, loaded in out-of-plane bending LA LB LC LD LE LF LG LH LI LJ 8.8 7.3 -0.6 0.3 9.1 -0.3 1.1 0.4 0.3 -0.4 LAB LAC LAD LAE LAF LAG LAH LAI LAJ LBC 2.1 0.9 0.1 2.7 -0.1 -1.0 0.2 0.2 1.0 -0.7 LBD LBE LBF LBI LBJ LCD LCE LCF LCG LCH 0.4 2.1 0.1 -0.1 -0.1 0.1 0.4 0 -0.4 0 LCI LCJ LDE LDF LDG LDH LEF LEG LEH LEI 0.1 1.4 -0.1 -0.1 -0.2 -0.1 0.2 0 0.3 -0.4 LEJ LFG LFH LFI LFJ LGI LGJ LHI LHJ 1.8 -0.3 0.2 0.5 0.1 0.1 0.2 -0.1 -0.4 99 Table 32: Aliased effects for re-analysis as a 26-1 of Layup 3, [(-45/45)2]s, loaded in out-ofplane bending LA LB LC LE LG LJ LAB LAC LAE LAG 8.8 7.3 -0.6 9.1 1.1 -0.4 2.1 0.9 2.7 -1.0 LAJ LBC LBE LBJ LCE LCG LCJ LEG LEJ LGJ 1.0 -0.7 2.1 -0.1 0.4 -0.4 1.4 0 1.8 0.2